Tips & Tricks
Analysis of polymer polymethyl metha-acralyte and single-wall cnt composites
Like this document? Why not share!
E – commerce adoption by micro smal...
Impact of fishing harbour on the li...
How does a work environment affect ...
Factors affecting the adoption of i...
Marketing strategies and practices ...
Minerals the wealth on earth
Email sent successfully!
Show related SlideShares at end
Analysis of polymer polymethyl metha-acralyte and single-wall cnt composites
Mar 02, 2013
Comment goes here.
12 hours ago
Are you sure you want to
Your message goes here
Be the first to comment
Be the first to like this
Number of Embeds
No notes for slide
Analysis of polymer polymethyl metha-acralyte and single-wall cnt composites
1. International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 – INTERNATIONAL JOURNAL OF ADVANCED RESEARCH IN 6480(Print), ISSN 0976 – 6499(Online) Volume 4, Issue 1, January- February (2013), © IAEME ENGINEERING AND TECHNOLOGY (IJARET)ISSN 0976 - 6480 (Print)ISSN 0976 - 6499 (Online) IJARETVolume 4, Issue 1, January- February (2013), pp. 28-34© IAEME: www.iaeme.com/ijaret.asp ©IAEMEJournal Impact Factor (2012): 2.7078 (Calculated by GISI)www.jifactor.com ANALYSIS OF POLYMER POLYMETHYL-METHA-ACRALYTE AND SINGLE-WALL CNT COMPOSITES FOR NEXT GENERATION ISSUES A.Saravananpandi Solairajana, Dr.G.Kalivarathanb a Research Scholar, CMJ University, Meghalaya, Shillong. b Principal/ PSN Institute of Technology and Science, Tirunelveli, Tamilnadu, Supervisor, CMJ university, Shillong. Email:email@example.com ABSTRACT Carbon nanotubes (CNTs) are normally having outstanding electrical, mechanical, optical, and thermal properties with significant importance in a wide range of applications such as quantum wires, tips for scanning probe microscope, and molecular diodes. A polymer plays an important role in various fields due to their advantages in lightness, ease of processing, resistance to corrosion, and low cost production. To improve the performance of polymers, composites of polymers and filler, namely micron-scale aggregate or fibers, have been extensively used and studied. The use of nano-scale fillers such as metals, semiconductors, organic and inorganic particles, and fibers, especially carbon structures, are of particular interest and the subject of intense investigation. The unique properties of carbon nanotubes offer crucial advantages over other nano fillers. The potential of using carbon nanotubes as filler in polymer composite has not been fully realized because of processing difficulties. Currently, there are only a few carbon nanotube-based, commercial products on the market with improved electrical conductivity. Thermal management such as heat removal from ICs is a critical problem that limits potential miniaturization, speed and reliability of micro electronics. For most modern microelectronic devices, cooling is restricted by the thermal conductivity of the polymeric packaging materials, since polymers typically have low thermal conductivity as compared to other materials. To enhance the thermal conductivity of polymers, fillers with higher thermal conductivity is required. The thermal conductivities of composites (polymer+fillers) is controlled by (i) filler concentration, (ii) filler conductivity, (iii) filler geometry, (iv) interface conductance between filler and polymer, and (v) homogeneity of the filler dispersion. The small particle sizes of nano fillers are expected to disperse more homogeneously within a polymer host than larger micro/milli-fillers. However, there remain serious gaps in the fundamental understanding of the interaction between nano- fillers and polymers that lead to the properties of the composite materials. 28
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 –6480(Print), ISSN 0976 – 6499(Online) Volume 4, Issue 1, January- February (2013), © IAEME1.0 INTRODUCTION Relaxation processes in amorphous materials are particularly important tounderstanding macroscopic properties. Calorimetry has revealed enthalpic relaxationsoccurring near the glass transition Tg in polymers aged after a variety of heating treatments.It is well known that annealing or variation of heating and cooling rates leads to significanthysteresis in Tg because of structural relaxations. The introduction of nano-fillers is expectedto strongly influence these short-range structural relaxations. However, the effectiveutilization of CNTs in polymer composite applications strongly depends upon thequality/uniformity of the nanotubes and the ability to disperse them homogeneouslythroughout the polymer host. Thus, the main objective of this work is to produce andinvestigate polymer+Single-wall CNT (SWCNT) nano composites materials, which arecandidates for next-generation of high-strength, light weight, and enhanced thermalconducting materials. This report describes a simple yet effective method to controllablydisperse SWCNTs in the polymer polymethyl-metha-acralyte (PMMA) and presents adetailed calorimetric study using modulation (ACC) and modulation-differential-scanning(MDSC) calorimetric techniques. The PMMA+SWCNT composites were prepared bydispersing SWCNTs and PMMA in a chloroform solution using sonication then slowlyevaporating the chloroform leaving a homogeneous dispersion. The specific heat andeffective thermal conductivity of the composites were determined by ACC from 300 to 400 Kas a function of SWCNT content. An enhancement of the effective thermal conductivity isobserved as the mass fraction of SWCNTs (φm) increases from 0.014 to 0.083. Theseexperimental results are in good agreement with a simple geometric model at low SWCNTcontent but are better described by more sophisticated models above φm = 0.034. The glasstransition dynamics of pure PMMA and PMMA+SWCNT samples were studied by MDSC asa function of temperature scan rate. The hysteresis between heating and cooling of thereversible specific heat decreases with decreasing scan rate for pure PMMA but is essentiallyunchanged in the composites, indicating the SWCNT may be quenching glassy structuraldynamics. In all samples, the effective glass transition temperature, Tg increases withincreasing scan rate (though less so for higher φm SWCNTs) but the MDSC determined Tgare consistently below the scattered values determined by the ACC method. This discrepancyis attributed to the effect of prolonged heat treatment of the composite for the ACCmeasurements. Following this introduction, the experimental procedures for the calorimetricmethods and sample preparation and this again follow results and discussion with theoreticalmodels for thermal conductivity in composite systems. A general conclusion in the enddescribes future directions.2.0 MODULATION CALORIMETRY In the ACC technique, the sample and cell, loosely coupled to a constant thermal bath,are subjected to a small oscillatory heat input. The specific heat and the effective thermalconductivity can be determined by measuring the frequency dependence of the amplitude andphase of the resulting temperature oscillation. The heat input, P0e−!t with P0 ≈ 0.5 mW, issupplied to the sample+cell and typically results in a modulated temperature having anamplitude Tac ≈ 5 mK. In the sample+cell “sandwich” or “stack” arrangement used in thisstudy, the total measured heat capacity is written as C = Cs+Cc, where Cs is the heat capacityof the PMMA or PMMA+SWCNT composite sample and Cc is the heat capacity of cell. Thecell heat capacity consists of Cc = CH + CAg + CGE, where CH is the heater, CAg is the 29
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 –6480(Print), ISSN 0976 – 6499(Online) Volume 4, Issue 1, January- February (2013), © IAEMEsilver sheets, and CGE is the GE varnish (used to attach all the components) contribution.The heat capacity of the PMMA or PMMA+SWCNT composite is Cs = C − Cc and specificheat capacity determined as Cp = Cs/ms, where ms is the mass of the sample. Thecontribution of the carbon-flake thermister, used to measure the temperature, is smallcompared to all other components and is neglected.The ACC experimental procedure details can be found elsewhere and the method to estimatethe effective thermal conductivity can be found. The effective thermal conductance Ks inunits ofWK−1, the inverse of the thermal resistance, of the sample is given bywhere τe = ReCs is the external thermal relaxation time constant, Re the external thermalresistance, ω the oscillatory frequency, and φ =θ+ π/2 is determined from the phase shiftbetween the heat input and resulting temperature change. With the geometric dimensions ofsample+cell configuration, the effective thermal conductivity κs in units of W m−1 K−1 can becalculated directly as κs = KsL/A, where L is the thickness and A is the cross-sectional areaof the sample. High-resolution ACC was performed using a home-built calorimeter. Thegeneral sample+cell configuration consisted of a “sandwich” or “stack” arrangement ofheater, thin silver sheet (0.1 mm thick, 5 mm square), PMMA/SWCNT/PMMA+SWCNTsample, thin silver sheet, and thermistor, all held together by thin applications of GE varnish.Here, the two silver sheets do not directly contact each other. The sample area closelymatches the dimensions of the heater attached to one silver sheet. A 120 strain-gauge heateris attached to one side of the “stack” and a 1 M carbon-flake thermistor to the other side byGE varnish. The sample was kept inside a thermal bath maintained at a controlled fixedtemperature. By supplying an oscillating voltage to the heater, small temperature oscillationsare induced in the sample+cell detected by the thermister. Scanning temperature isaccomplished by changing the bath temperature. The resolution of the sample+cell and bathtemperatures are in µK range. Modulated (temperature) differential scanning calorimetry(MTDSC/MDSC) allows for simultaneous measurements of the heat flow and heat capacity.This is a more refined version of the conventional DSC method. MDSC differs fromconventional DSC in that the sample is subjected to a more complex heating program,incorporating a sinusoidal temperature modulation onto an underlying linear heating ramp.Whereas DSC is only capable of measuring the total heat flow, MDSC can simultaneouslydetermine the nonreversible (kinetic component) and the reversible (heat capacitycomponent) heat flows. In this MDSC technique, the reversible heat capacity signal wasdetermined automatically by integrating the total heat flow rates over time. A detaileddescription of the MDSC method can be found elsewhere. The MDSC experiment wasperformed using a Model Q200 MDSC from TA Instruments, Inc. Samples were heated for15 min at 127 0C in vacuum to remove any trapped chloroform, prior to mounting in theMDSC, and subjected to underlying heating and cooling rates of 10, 5, 1, 0.5, and 0.1 K/minand a temperature modulation amplitude of 0.6 K with a period of 60 s. Dry ultra pureNitrogen gas was purged through the sample holder in a rate of 50 ml/min during theexperiment. 30
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 –6480(Print), ISSN 0976 – 6499(Online) Volume 4, Issue 1, January- February (2013), © IAEME3.0 PREPARATION OF PMMA+SWCNT COMPOSITES The polymer PMMA (Mn = 120, 000 g mol−1, obtained from Aldrich) was firstdissolved in a dilute chloroform solution. The required amount of SWCNTs (Helix MaterialsSolutions, TX, purity > 90 %, ash ≈ 5 %) was also dispersed into a dilute chloroform solutionand sonicated for 12 hr to separate the bundles of nanotubes into individual particles.Scanning electron micrographs of the SWCNT material used in this work, presented in aprevious report, found the diameter to be 1.3 nm and the length varying from 0.5 to 50 µm.Both the PMMA+chloroform dilute solution and the SWCNT dispersed in chloroformsolution were then mixed together and again kept ≈ 6 hr in an ultrasonic bath. After thePMMA+SWCNT+chloroform dilute solution was finally mixed with a touch mixer (FisherTouch-Mixer model 12-810) for 10 mins, no detectable precipitation was observed.Immediately after this final mixing, the solution was drop cast onto a thin silver sheet to forma thin film of PMMA+SWCNT and placed for 6 hrs undervacuum to remove the chloroform. The typical thickness of the sample film is between 150 to200 µm. The sample was then sandwiched between two thin silver sheets with GE varnishand again dried under vacuum to remove any solvents from the varnish. Figure 1: A: Mixture of PMMA and SWCNTs composites before dispersion, B: just after dispersion, C: after one day of dispersion, D: after two days dispersion and E: after 5 days of dispersion. F: is the optical micrograph images shows poor quality of dispersion, which was taken without sufficient time of sonication and mixing with touch mixture, G: shows the good quality of dispersion of SWCNTs inside PMMA with sufficient time of dispersion and then with touch mixture.All samples have essentially the same thickness and cross-sectional areas. Thus, the thermalcontact resistance of all samples are approximately same and should not play a role incomparing results as a function of SWCNT content. For the MDSC measurements, thesamples were sealed inside a standard hermite pan. The mass of the sample pan and referencepan was very close to each other to minimize the uncertainty of measurement. 31
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 –6480(Print), ISSN 0976 – 6499(Online) Volume 4, Issue 1, January- February (2013), © IAEME4.0 RESULTS AND DISCUSSION The specific heat of all samples exhibits similar temperature dependence from ≈ 300to 400 K with only a small change in its absolute value. Since φm is small, Cp is not expectedto vary substantially and so these results more reflect the reproducibility of the absolute valueof Cp measurements by the ACC technique. The experimental Cp value for pure PMMA isfound to be 1.61 J g−1 K−1, about 10 % above the literature value and within 18 % at 307 Kof the value Specific heat values of pure PMMA and PMMA+SWCNT composites at 300 K(glass state) and 399 K (liquid state). The Cp values of PMMA+SWCNT composites varyslightly from pure PMMA at room temperature and in a manner similar to that reported forcomposites of nanotubes dispersed in polystyrene. The variation of Cp values betweenPMMA and PMMA+SWCNT composites is likely due to experimental uncertainty,especially in the mass measurements of the sample+cell components. Figure 2: The effective specific heat (top panel) and thermal conductivity (bottom panel) of pure PMMA and five PMMA+SWCNTs composite samples from 300 to 400 K. See legend. In lower panel, the definition of the effective thermal conductivity increase between the glass and liquid state δκ is presented.the effective thermal conductivity κ using ACC of pure PMMA and PMMA+SWCNTsamples from φm = 0.014 to 0.083. The effective thermal conductivity was derived from theheat capacity measurements and frequency scans performed at regular temperature intervals,the details of the experimental derivation of κ can be found elsewhere. The effective κ forpure PMMA was found to be 0.172 W m−1 K−1 at 300 K and increases with temperaturerevealing a step-like feature near and about the glass transition. The absolute value of thederived κ is within 14 % at 307 K and 9 % at 352 K of the literature value for pure PMMAThe effect of a homogeneous random dispersion can be crucial because once the nanotubeconcentration increases, the nanotubes tendency to bundle increases. Once bundles form, thethermal pathways through a network of SWCNT become ’jammed’ resulting in a moremodest increase in κ. The influence of the nanotube geometry, average length and diameter, 32
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 –6480(Print), ISSN 0976 – 6499(Online) Volume 4, Issue 1, January- February (2013), © IAEMEon the thermal conductivity of the composite can also be large since these factors directlyinfluence the packing fraction of SWCNT that in turn plays an important role in theenhancement of the thermal conductivity. Also, the diameter of the nanotube is importantbecause, in general, the contact resistance decreases with increasing CNT diameter due to thelarger contact area in addition to the increase in the number of contacts per unit volume. Thethermal boundary resistance between carbon nanotubes and polymer/liquid environmentcomposites has been simulated and indicate large local temperature gradients as a function ofdistances from the nanotube long axis with constant radial heat flow. It was estimated that thetemperature decreases 40 % just 20 0A away from the long axis of the nanotubes, in thepolymer-liquid interface region. This particular simulation result suggests that largeEnhancement of κ in these composites would only be expected for samples with small meandistance between CNTs, hence high φm. Figure 3: Log-log plot of the percent enhancement of the thermal conductivity,κ from pure PMMA (top panel) and the change in thermal conductivity δκ (bottom panel) of PMMA+SWCNT composites between the glass (300 K) and liquid states (399 K), as a function of SWCNT mass fraction φm. Arrow indicates the δκ for pure PMMA5.0 CONCLUSION This work presents a detailed calorimetric study of the specific heat and effectivethermal conductivity of a macroscopic arrangement of randomly dispersed SWCNTs inside apolymer host. Using ACC and MDSC techniques, the enhancement of the effective thermalconductivity is significant with increased loading of SWCNTs. Higher thermal conductivityof polymer+CNT composites can be achieved by using suitable dispersion methods andhigher quality nanofiller materials. The glass transition characteristics, thermal conductivity,electrical conductivity, and mechanical properties of polymer composites can be controlledby adjusting the properties of the nanofillers. The increase in κ with increasing φm ofSWCNT is consistent with essentially independent particles for low concentration that is 33
International Journal of Advanced Research in Engineering and Technology (IJARET), ISSN 0976 –6480(Print), ISSN 0976 – 6499(Online) Volume 4, Issue 1, January- February (2013), © IAEMEdescribable by a simple Geometric model. For SWCNT higher than φm ൌ0.034, a model thattakes into account the packing fraction as well as nanoparticle shape is needed and indicatesthe onset of interactions among SWCNT, suggesting the presence of a spanning network. Theincrease in the zero-scan rate glass transition temperature and suppression of the enthalpichysteresis supports the view that the random inclusions of SWCNT in PMMA quenchesstructural relaxations and stabilizes the glass state. Continued experimental study, specificallyby rheological techniques, is required for these types of complex composite systems as wellas a more comprehensive modeling to properly understand and calibrate/engineer themacroscopic properties.REFERENCES S. J. Tans, M. H. Devoret, H. Dai, A. Theses and R. E. Smalley, Nature., 386, 474 (1997). H. Dai, J. H. Hafner, A. G. Rinzler, D. T. Colbert, and R. E. Smalley, Nature., 384, 147(1996). S. J. Sander, J. Tans, A. R. M. Verschueren, and C. Dekker, Nature., 393, 49 (1999). Ijima Sumio, Helical microtubules of graphitic carbon,Nature., 354, 8, No.56 (1991). S. Glushanin, V. Y. Topolov, and A. V. Krivoruchko, Materials Chemistry and Physics.,97, 357 (2006). P. Hine, V. Broome, and I. Ward, Polymer., 46, 10935 (2005). N. Cioffi, L. Torsi, N. Ditaranto, G. Tantillo, L. Ghibelli, L. Sabbatini, T. BleveZacheo,M. D. Alessio, P. G. Zambonin, and E. Traversa, Chemistry of Materials.,317, 5255 (2005). A. Pelaiz-Barranco and P. Marin-Franch, J. Appl. Phys., 97, 034104 (2005). A. Bar-Cohen, A. Watwe, and K. N. Seetharamu, Fundamentals of Thermal Managementin Fundamentals of Microsystems Packaging, Chapter 6, Ed., R.R. Tummala, McGraw Hill,New York (2001). B. Wunderlich, Thermal Analysis of Polymeric Materials. Springer-Velag: Berlin,Heidelberg, (2005). B. Wunderlich, Thermal analysis. New York: Academic Press., 135, 205 (1990). M. Meyyappan, Carbon nanotubes science and applications, CRC Press: Boca Raton, FL(2005). P. J. F. Harris, Carbon nanotubes and related structures new materials for the twenty-firstcentury;Cambridge University Press: Cambridge (2001). www.pageout.net/user/www/l/y/lyee/specificheat.pdf. M. J. Assael, S. Botsios, K. Gialou and N. Metaxa,International Journal of Ther-mophysics,26, ,1995 (2005). C. Rauwendal,Polymer Extrusion,PUBLISHER - HanserMunich, GDR (1986). S. Agarwal, M. Mashud, K. Khan, and R. K. Gupta, Polymer Eng and Science., 129, 1(2008). Y. Yang, M. C. Gupta, J. N. Zalameda and W. P. Winfree, Micro and Nano Letters, 3,No.2, 35-40 (2008). L. E. Nielsen, Ind. Eng. Chem. Fundam., 13, 17 (1974). R. L. Hamilton and O. K. Crosser, Ind. Eng. Chem. Fundamen., 1, 187 (1962). 34
Email sent successfully..